#------------------------------------------------------------------------------
#$Date: 2025-07-01 13:47:20 +0300 (Tue, 01 Jul 2025) $
#$Revision: 1123 $
#$URL: svn://crystallography.net/testcod/cif/7/10/00/7100003.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7100003
loop_
_publ_author_name
'Jones, Richard H.'
'Bull, Craig L.'
'Funnell, Nicholas P.'
'Knight, Kevin S.'
'Marshall, William G.'
_publ_section_title
;
 Exploring the full range of N⋯I⋯X halogen-bonding
 interactions within a single compound using pressure
;
_journal_issue                   35
_journal_name_full               'Chemical Communications'
_journal_page_first              4663
_journal_page_last               4666
_journal_paper_doi               10.1039/D4CC00847B
_journal_volume                  60
_journal_year                    2024
_chemical_formula_sum            'C3 Cl D9 I N'
_chemical_formula_weight         230.52
_space_group_IT_number           61
_space_group_name_Hall           '-P 2ac 2ab'
_space_group_name_H-M_alt        'P b c a'
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_H-M   'P b c a'
_audit_update_record
;
2024-02-08 deposited with the CCDC.	2024-03-26 downloaded from the CCDC.
;
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            8
_cell_length_a                   10.7993(30)
_cell_length_b                   10.2187(32)
_cell_length_c                   9.9564(30)
_cell_measurement_temperature    250
_cell_volume                     1098.7(6)
_diffrn_ambient_temperature      250
_pd_block_id
2023-07-06T21:07|PRL67235_38_50TNS_25_phase1|WGM||
_pd_phase_name                   'TMEICl H-calc.cif'
_cod_data_source_file            d4cc00847b2.cif
_cod_data_source_block           PRL67235_38_50TNS_25_phase_1
_cod_original_cell_volume        1098.73(31)
_cod_original_formula_sum        'C3 D9 Cl I N'
_cod_database_code               7100003
_diffrn_measurement_pressure     4341000
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 -x+1/2,+y+1/2,+z
3 +x,-y+1/2,+z+1/2
4 -x+1/2,-y,+z+1/2
-1 -x,-y,-z
-2 +x+1/2,-y+1/2,-z
-3 -x,+y+1/2,-z+1/2
-4 +x+1/2,+y,-z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
N N 0.2038(17) 0.0366(16) 0.2651(18) 1.0 Uiso 0.018(5) 8
C C1 0.2670(16) 0.1363(16) 0.3471(17) 1.0 Uiso 0.018(5) 8
C C2 0.3031(19) -0.0438(19) 0.2048(19) 1.0 Uiso 0.018(5) 8
C C3 0.1255(15) -0.0413(18) 0.3566(18) 1.0 Uiso 0.018(5) 8
D D1 0.325(4) 0.1894(29) 0.2878(35) 1.0 Uiso 0.0103(34) 8
D D2 0.1971(30) 0.202(4) 0.3930(33) 1.0 Uiso 0.0103(34) 8
D D3 0.3180(32) 0.0902(27) 0.423(4) 1.0 Uiso 0.0103(34) 8
D D4 0.3629(34) 0.0173(34) 0.147(4) 1.0 Uiso 0.0103(34) 8
D D5 0.2585(31) -0.124(4) 0.134(4) 1.0 Uiso 0.0103(34) 8
D D6 0.3516(29) -0.0875(34) 0.2777(33) 1.0 Uiso 0.0103(34) 8
D D7 0.1830(29) -0.092(4) 0.427(4) 1.0 Uiso 0.0103(34) 8
D D8 0.0613(35) 0.0245(35) 0.411(4) 1.0 Uiso 0.0103(34) 8
D D9 0.0715(33) -0.1135(34) 0.2976(33) 1.0 Uiso 0.0103(34) 8
I I 0.111(4) 0.127(4) 0.104(5) 1.0 Uiso 0.010(5) 8
Cl Cl -0.0440(26) 0.2392(28) -0.0822(27) 1.0 Uiso 0.010(5) 8
loop_
_atom_type_symbol
_atom_type_number_in_cell
N 8.0
D 72.0
C 24.0
I 8.0
Cl 8.0
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
C1 N C2 105.8(14) 1_555 . 1_555 N
C1 N C3 107.3(14) 1_555 . 1_555 N
C1 N I 109.9(17) 1_555 . 1_555 N
C2 N C3 111.5(14) 1_555 . 1_555 N
C2 N I 106.1(17) 1_555 . 1_555 N
C3 N I 115.8(18) 1_555 . 1_555 N
N C1 D1 109.45(22) 1_555 . 1_555 N
N C1 D2 109.46(22) 1_555 . 1_555 N
N C1 D3 109.46(22) 1_555 . 1_555 N
D1 C1 D2 109.48(22) 1_555 . 1_555 N
D1 C1 D3 109.49(22) 1_555 . 1_555 N
D2 C1 D3 109.48(22) 1_555 . 1_555 N
N C2 D4 109.44(22) 1_555 . 1_555 N
N C2 D5 109.46(22) 1_555 . 1_555 N
N C2 D6 109.47(22) 1_555 . 1_555 N
D4 C2 D5 109.49(22) 1_555 . 1_555 N
D4 C2 D6 109.49(22) 1_555 . 1_555 N
D5 C2 D6 109.48(22) 1_555 . 1_555 N
N C3 D7 109.46(22) 1_555 . 1_555 N
N C3 D8 109.44(22) 1_555 . 1_555 N
N C3 D9 109.47(22) 1_555 . 1_555 N
D7 C3 D8 109.48(22) 1_555 . 1_555 N
D7 C3 D9 109.47(22) 1_555 . 1_555 N
D8 C3 D9 109.50(22) 1_555 . 1_555 N
N I Cl 170.7(24) 1_555 . 1_555 N
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
N C1 1.474(9) . 1_555 N
N C2 1.478(9) . 1_555 N
N C3 1.475(9) . 1_555 N
N D1 2.052(34) . 1_555 N
N D2 2.121(34) . 1_555 N
N D3 2.07(4) . 1_555 N
N D4 2.089(33) . 1_555 N
N D5 2.18(4) . 1_555 N
N D6 2.043(30) . 1_555 N
N D7 2.093(32) . 1_555 N
N D8 2.119(35) . 1_555 N
N D9 2.121(35) . 1_555 N
N I 2.10(5) . 1_555 N
C1 N 1.474(9) . 1_555 N
C1 D1 1.02(5) . 1_555 N
C1 D2 1.11(4) . 1_555 N
C1 D3 1.05(5) . 1_555 N
C1 D4 2.551(34) . 1_555 N
C1 D5 2.87(4) . 4_555 N
C1 D6 2.558(33) . 1_555 N
C1 D7 2.625(35) . 1_555 N
C1 D7 2.94(4) . 2_555 N
C1 D8 2.58(4) . 1_555 N
C1 I 2.95(4) . 1_555 N
C2 N 1.478(9) . 1_555 N
C2 D1 2.533(31) . 1_555 N
C2 D3 2.57(4) . 1_555 N
C2 D4 1.06(4) . 1_555 N
C2 D5 1.19(5) . 1_555 N
C2 D6 1.00(4) . 1_555 N
C2 D7 2.614(33) . 1_555 N
C2 D7 3.09(4) . 4_554 N
C2 D8 3.10(4) . -4_555 N
C2 D9 2.76(4) . 1_555 N
C2 D9 2.98(4) . -4_555 N
C2 I 2.89(5) . 1_555 N
C3 N 1.475(9) . 1_555 N
C3 D1 2.886(32) . 2_545 N
C3 D2 2.63(4) . 1_555 N
C3 D3 2.56(4) . 1_555 N
C3 D4 2.91(4) . 4_555 N
C3 D4 2.90(4) . -4_455 N
C3 D5 2.77(4) . 1_555 N
C3 D6 2.608(30) . 1_555 N
C3 D7 1.07(4) . 1_555 N
C3 D8 1.11(4) . 1_555 N
C3 D8 3.07(4) . -1_556 N
C3 D9 1.11(4) . 1_555 N
D1 N 2.052(34) . 1_555 N
D1 C1 1.02(5) . 1_555 N
D1 C2 2.533(31) . 1_555 N
D1 C3 2.886(32) . 2_555 N
D1 D2 1.74(5) . 1_555 N
D1 D3 1.69(5) . 1_555 N
D1 D4 2.28(4) . 1_555 N
D1 D5 3.63(5) . 1_555 N
D1 D5 2.61(5) . 2_555 N
D1 D5 3.62(6) . 4_555 N
D1 D6 2.85(4) . 1_555 N
D1 D6 2.98(5) . 2_555 N
D1 D7 3.54(5) . 1_555 N
D1 D7 2.63(5) . 2_555 N
D1 D7 3.73(5) . 4_554 N
D1 D8 3.53(6) . 1_555 N
D1 D8 3.84(5) . 2_555 N
D1 D8 3.64(5) . -4_555 N
D1 D9 2.30(4) . 2_555 N
D1 I 3.02(5) . 1_555 N
D1 I 3.33(5) . -4_555 N
D1 Cl 2.59(5) . -2_555 N
D1 Cl 3.29(4) . -4_555 N
D2 N 2.121(34) . 1_555 N
D2 C1 1.11(4) . 1_555 N
D2 C3 2.63(4) . 1_555 N
D2 D1 1.74(5) . 1_555 N
D2 D3 1.76(5) . 1_555 N
D2 D3 3.98(4) . 2_555 N
D2 D4 3.57(5) . 1_555 N
D2 D4 3.45(5) . 4_555 N
D2 D5 3.16(5) . 2_555 N
D2 D5 2.57(5) . 4_555 N
D2 D6 3.59(5) . 1_555 N
D2 D6 2.49(5) . 2_555 N
D2 D7 3.03(5) . 1_555 N
D2 D7 2.49(5) . 2_555 N
D2 D8 2.34(5) . 1_555 N
D2 D9 3.63(5) . 1_555 N
D2 D9 3.27(5) . 2_555 N
D2 D9 3.94(6) . -3_555 N
D2 I 3.12(5) . 1_555 N
D2 I 2.88(6) . 3_555 N
D2 Cl 2.68(5) . 3_555 N
D2 Cl 3.39(4) . -4_555 N
D3 N 2.07(4) . 1_555 N
D3 C1 1.05(5) . 1_555 N
D3 C2 2.57(4) . 1_555 N
D3 C3 2.56(4) . 1_555 N
D3 D1 1.69(5) . 1_555 N
D3 D2 1.76(5) . 1_555 N
D3 D2 3.98(4) . 2_545 N
D3 D4 2.89(5) . 1_555 N
D3 D4 3.16(6) . 4_555 N
D3 D5 3.68(5) . 1_555 N
D3 D5 2.28(5) . 4_555 N
D3 D6 2.35(4) . 1_555 N
D3 D6 3.98(5) . 4_555 N
D3 D7 2.36(4) . 1_555 N
D3 D7 3.25(5) . 2_555 N
D3 D8 2.86(5) . 1_555 N
D3 D9 3.60(5) . 1_555 N
D3 D9 3.49(5) . 2_555 N
D3 D9 3.92(6) . 4_555 N
D3 I 2.95(6) . 4_555 N
D3 I 3.20(6) . -4_555 N
D3 Cl 2.65(4) . -4_555 N
D4 N 2.089(33) . 1_555 N
D4 C1 2.551(34) . 1_555 N
D4 C2 1.06(4) . 1_555 N
D4 C3 2.91(4) . 4_554 N
D4 C3 2.90(4) . -4_555 N
D4 D1 2.28(4) . 1_555 N
D4 D2 3.57(5) . 1_555 N
D4 D2 3.45(5) . 4_554 N
D4 D3 2.89(5) . 1_555 N
D4 D3 3.16(6) . 4_554 N
D4 D5 1.84(5) . 1_555 N
D4 D5 3.89(5) . 2_555 N
D4 D6 1.69(5) . 1_555 N
D4 D7 3.58(5) . 1_555 N
D4 D7 2.37(5) . 4_554 N
D4 D7 3.71(5) . -4_555 N
D4 D8 2.53(5) . 4_554 N
D4 D8 2.22(5) . -4_555 N
D4 D9 3.73(5) . 1_555 N
D4 D9 3.69(5) . 4_554 N
D4 D9 2.68(5) . -4_555 N
D4 I 2.97(6) . 1_555 N
D4 I 3.82(6) . -4_555 N
D4 Cl 2.76(5) . -2_555 N
D5 N 2.18(4) . 1_555 N
D5 C1 2.87(4) . 4_554 N
D5 C2 1.19(5) . 1_555 N
D5 C3 2.77(4) . 1_555 N
D5 D1 3.63(5) . 1_555 N
D5 D1 2.61(5) . 2_545 N
D5 D1 3.62(6) . 4_554 N
D5 D2 3.16(5) . 2_545 N
D5 D2 2.57(5) . 4_554 N
D5 D3 3.68(5) . 1_555 N
D5 D3 2.28(5) . 4_554 N
D5 D4 1.84(5) . 1_555 N
D5 D4 3.89(5) . 2_545 N
D5 D6 1.79(5) . 1_555 N
D5 D7 3.05(5) . 1_555 N
D5 D7 3.65(6) . 3_544 N
D5 D7 3.08(6) . 4_554 N
D5 D8 3.80(6) . 1_555 N
D5 D8 3.12(5) . 4_554 N
D5 D8 3.63(5) . -4_555 N
D5 D9 2.60(5) . 1_555 N
D5 D9 3.45(5) . -4_555 N
D5 I 3.03(6) . 1_555 N
D5 I 2.92(6) . 2_545 N
D5 Cl 2.65(6) . -1_555 N
D6 N 2.043(30) . 1_555 N
D6 C1 2.558(33) . 1_555 N
D6 C2 1.00(4) . 1_555 N
D6 C3 2.608(30) . 1_555 N
D6 D1 2.85(4) . 1_555 N
D6 D1 2.98(5) . 2_545 N
D6 D2 3.59(5) . 1_555 N
D6 D2 2.49(5) . 2_545 N
D6 D3 2.35(4) . 1_555 N
D6 D3 3.98(5) . 4_554 N
D6 D4 1.69(5) . 1_555 N
D6 D5 1.79(5) . 1_555 N
D6 D7 2.35(4) . 1_555 N
D6 D7 3.96(5) . 4_554 N
D6 D8 3.59(5) . 1_555 N
D6 D8 3.83(5) . 4_554 N
D6 D8 3.16(5) . -4_555 N
D6 D9 3.04(5) . 1_555 N
D6 D9 2.50(5) . -4_555 N
D6 I 3.81(6) . 1_555 N
D6 I 3.42(6) . 2_545 N
D6 I 3.30(6) . 4_555 N
D6 I 3.75(6) . -4_555 N
D6 Cl 2.94(5) . 4_555 N
D7 N 2.093(32) . 1_555 N
D7 C1 2.625(35) . 1_555 N
D7 C1 2.94(4) . 2_545 N
D7 C2 2.614(33) . 1_555 N
D7 C2 3.09(4) . 4_555 N
D7 C3 1.07(4) . 1_555 N
D7 D1 3.54(5) . 1_555 N
D7 D1 2.63(5) . 2_545 N
D7 D1 3.73(5) . 4_555 N
D7 D2 3.03(5) . 1_555 N
D7 D2 2.49(5) . 2_545 N
D7 D3 2.36(4) . 1_555 N
D7 D3 3.25(5) . 2_545 N
D7 D4 3.58(5) . 1_555 N
D7 D4 2.37(5) . 4_555 N
D7 D4 3.71(5) . -4_455 N
D7 D5 3.05(5) . 1_555 N
D7 D5 3.65(6) . 3_545 N
D7 D5 3.08(6) . 4_555 N
D7 D6 2.35(4) . 1_555 N
D7 D6 3.96(5) . 4_555 N
D7 D8 1.78(5) . 1_555 N
D7 D8 3.17(5) . -1_556 N
D7 D9 1.78(5) . 1_555 N
D7 I 2.86(6) . 4_555 N
D7 Cl 2.760(34) . -3_545 N
D8 N 2.119(35) . 1_555 N
D8 C1 2.58(4) . 1_555 N
D8 C2 3.10(4) . -4_455 N
D8 C3 1.11(4) . 1_555 N
D8 C3 3.07(4) . -1_556 N
D8 D1 3.53(6) . 1_555 N
D8 D1 3.84(5) . 2_545 N
D8 D1 3.64(5) . -4_455 N
D8 D2 2.34(5) . 1_555 N
D8 D3 2.86(5) . 1_555 N
D8 D4 2.53(5) . 4_555 N
D8 D4 2.22(5) . -4_455 N
D8 D5 3.80(6) . 1_555 N
D8 D5 3.12(5) . 4_555 N
D8 D5 3.63(5) . -4_455 N
D8 D6 3.59(5) . 1_555 N
D8 D6 3.83(5) . 4_555 N
D8 D6 3.16(5) . -4_455 N
D8 D7 1.78(5) . 1_555 N
D8 D7 3.17(5) . -1_556 N
D8 D8 2.27(7) . -1_556 N
D8 D9 1.81(5) . 1_555 N
D8 D9 3.36(5) . -1_556 N
D8 I 3.28(6) . 1_555 N
D8 Cl 2.67(6) . 3_555 N
D8 Cl 3.38(4) . -3_545 N
D9 N 2.121(35) . 1_555 N
D9 C2 2.76(4) . 1_555 N
D9 C2 2.98(4) . -4_455 N
D9 C3 1.11(4) . 1_555 N
D9 D1 2.30(4) . 2_545 N
D9 D2 3.63(5) . 1_555 N
D9 D2 3.27(5) . 2_545 N
D9 D2 3.94(6) . -3_545 N
D9 D3 3.60(5) . 1_555 N
D9 D3 3.49(5) . 2_545 N
D9 D3 3.92(6) . 4_554 N
D9 D4 3.73(5) . 1_555 N
D9 D4 3.69(5) . 4_555 N
D9 D4 2.68(5) . -4_455 N
D9 D5 2.60(5) . 1_555 N
D9 D5 3.45(5) . -4_455 N
D9 D6 3.04(5) . 1_555 N
D9 D6 2.50(5) . -4_455 N
D9 D7 1.78(5) . 1_555 N
D9 D8 1.81(5) . 1_555 N
D9 D8 3.36(5) . -1_556 N
D9 I 3.15(6) . 1_555 N
D9 I 3.45(6) . -3_545 N
D9 Cl 2.52(5) . -1_555 N
D9 Cl 3.22(4) . -3_545 N
I N 2.10(5) . 1_555 N
I C1 2.95(4) . 1_555 N
I C2 2.89(5) . 1_555 N
I D1 3.02(5) . 1_555 N
I D1 3.33(5) . -4_455 N
I D2 3.12(5) . 1_555 N
I D2 2.88(6) . 3_554 N
I D3 2.95(6) . 4_554 N
I D3 3.20(6) . -4_455 N
I D4 2.97(6) . 1_555 N
I D4 3.82(6) . -4_455 N
I D5 3.03(6) . 1_555 N
I D5 2.92(6) . 2_555 N
I D6 3.81(6) . 1_555 N
I D6 3.42(6) . 2_555 N
I D6 3.30(6) . 4_554 N
I D6 3.75(6) . -4_455 N
I D7 2.86(6) . 4_554 N
I D8 3.28(6) . 1_555 N
I D9 3.15(6) . 1_555 N
I D9 3.45(6) . -3_555 N
I Cl 2.75(5) . 1_555 N
Cl D1 2.59(5) . -2_455 N
Cl D1 3.29(4) . -4_455 N
Cl D2 2.68(5) . 3_554 N
Cl D2 3.39(4) . -4_455 N
Cl D3 2.65(4) . -4_455 N
Cl D4 2.76(5) . -2_455 N
Cl D5 2.65(6) . -1_555 N
Cl D6 2.94(5) . 4_554 N
Cl D7 2.760(34) . -3_555 N
Cl D8 2.67(6) . 3_554 N
Cl D8 3.38(4) . -3_555 N
Cl D9 2.52(5) . -1_555 N
Cl D9 3.22(4) . -3_555 N
Cl I 2.75(5) . 1_555 N
loop_
_pd_block_diffractogram_id
2023-07-06T21:07|PRL67235_38_50TNS_25_H_01|WGM|PEARL
